Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236
Modelling And Optimization Of Process Parameters For Tig Welding Of Aluminium65032 Using Response Surface Methodology Palani.P.K1 , Saju.M2,
Associate Professor 1 , PG Scholar 2 Department of Mechanical Engineering, Government College of Technology, Coimbatore.
Abstract Tungsten inert gas welding is one of the widely used techniques for joining ferrous and non ferrous metals. TIG welding offers several advantages like joining of dissimilar metals, low heat affected zone, absence of slag etc. The aim of this paper is to investigate the effect of TIG welding process parameters on welding of Aluminium65032. Response Surface Methodology was used to conduct the experiments. The parameters selected for controlling the process are welding speed, current and gas flow rate. Strength of welded joints were tested by a UTM. Percent elongation was also calculated to evaluate the ductility of the welded joint. From the results of the experiments, mathematical models have been developed to study the effect of process parameters on tensile strength and percent elongation. Optimization was done to find optimum welding conditions to maximize tensile strength and percent elongation of welded specimen. Confirmation tests were also conducted to validate the optimum parameter settings.
Keywords: TIG welding, Al65032, Ultimate Tensile Strength, Response Surface Methodology.
1. INTRODUCTION 1.1 WELDING Welding is a fabrication process that joins materials, usually metals or thermoplastics by causing coalescence. Gas tungsten arc welding, GTAW, also known as tungsten inert gas welding, is an arc welding process that uses a non consumable electrode to produce the weld. Weld area is protected from atmospheric contamination by a shielding gas (usually inert gas such as argon) and a filler material is normally used.GTAW is most commonly used to weld thin sections of stainless steel and non ferrous metals such as aluminium, magnesium and copper alloys. Aluminium based alloys have been widely used in automobile structures due to their unique properties such as high strength to weight ratio. 1.2 Aluminium – 65032 Aluminium – 65032 is a precipitation hardening aluminium alloy [1], which has good mechanical
properties, exhibits good weld ability and is one of the most common alloys of aluminium. Chemical composition [1] of Al65032 is given in table 1 Table 1: Chemical composition of Aluminium – 65032 Al Si Fe Cu Mn Cr Zi Ti 97.53 0.4 <0.7 0.15 – <0.15 0.04 <0.25 <0.15 0.8 0.4 0.35 Application of Al – 65032 alloy includes construction of aircraft structures, construction of boats, bicycle frames and components, automobile parts, cans for packing of food stuffs and beverages etc.
2. LITERATURE REVIEW G.Haragopal et al. (2011) [1] used Taguchi method to study the effect of gas pressure,current,grooveangle and preheat on MIG welding of Aluminium alloy(Al65032). They indicated that welding current has more effect ultimate tensile strength whereas gas pressure is the most significant parameter for proof stress, elongation and impact energy. G.Padmanaban et al (2011) [2] studied the effect of optimization of pulsed current gas tungsten arc welding process parameters on tensile strength in AZ31B magnesium alloy. Result showed that maximum tensile strength of 188Mpa was obtained under the welding condition of peak current of 210 A, base current of 80A, pulse frequency of 6 Hz and pulse on time of 50%. R.Satish et al. (2012) [3] studied weldability and process parameter optimization of dissimilar pipe joints using GTAW. Taguchi method was used to formulate the experimental layout to rank the welding input parameters which affects quality of weld. Results showed that lower heat input resulted in lower tensile strength and too high heat input also resulted in reduced tensile strength. Dr.Kumar et al (2009) [4] investigated the effect of process parameters on GTAW for Al7039 alloy. Taguchi method is used to formulate the experimental layout to analyze the effect of each process parameters on bead geometry. Narongchai Sathavornvichit et al, (2006) [5] determined the optimal factors of Flux cored arc welding process for steel ST37.Experiments were conducted by central composite design,They found
230  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236
3. METHODOLOGY INVESTIGATION
OF
3.1 Response Surface Methodology (RSM) Response Surface Methodology (RSM) is a collection of statistical and mathematical techniques useful for developing, improving, and optimizing processes [2, 1011]. With this technique, the effect of two or more factors on quality criteria can be investigated and optimum values are obtained. In RSM design there should be at least three levels for each factor.
Table 2: Factors & Levels Levels Factors
Notation
that optimum conditions were 300ampere of current,30volt of voltage,45mm of stickout and 60 degrees of angle. Ugur esme et al.(2009) [6] investigated the multi response optimization of tungsten inert gas welding for an optimal parametric combination to yield favorable bead geometry of welded joints using grey relational analysis and Taguchi method. The significance of factors on overall quality characteristics of the weldment has also been evaluated quantitatively by the analysis of variance method. M.Balasubramanian et al (2009) [7] studied the weld pool geometry of pulsed current gas tungsten arc welded titanium alloy using central composite design. Mathematical models were developed. Lexicographic method was used to optimize process parameters. Erdal Karadeniz et al (2007) [8] studied the effects of various welding parameters on welding penetration in ERD emir 6842 steel having 2.5mm thickness welded by robotic gas metal arc welding. welding current ,welding speed and arc voltage were chosen as process parameters. The depth of penetration were measured for each specimen and effect of these parameters on penetration were researched. From the study, it is found that increasing welding current increased the depth of penetration. D.S.Nagesh et al (2002) [9] studied that bead geometry and penetration are important physical characteristic of a weldament. It was observed that high arc travel rate or low arc power normally produce poor fusion. A neural network was developed for estimating weld bead and penetration geometric parameters. From the literatures, it is observed that only few works have been reported on the study of TIG welding process parameters for welding of Aluminium65032. Therefore the aim of the present study is to investigate the effect of TIG welding process parameters on the welding of Al65032.The experiments were conducted using a statistical technique called Design of Experiments (DOE).
1
0
+1
Welding speed (mm / S 150 175 200 min) Welder current (Amps) I 100 110 120 Gas flow rate (LPM) L 10 11 12 RSM also quantifies relationships among one or more measured responses and the vital input factors. The version 14 of the MINITAB software was used to develop the experimental plan for RSM. 3.2 Central Composite Design (CCD) The first requirement for RSM involves the design of experiments to achieve adequate and reliable measurement of the response of interest. To meet this requirement, an appropriate experimental design technique has to be employed. The experimental design techniques commonly used for process analysis and modelling are the full factorial, partial factorial and central composite designs. A full factorial design requires at least three levels per variable to estimate the coefficients of the quadratic terms in the response model A partial factorial design requires fewer experiments than the full factorial design However, the former is particularly useful if certain variables are already known to show no interaction. An effective alternative to factorial design is central composite design (CCD), [5, 1314] requires many fewer tests than the full factorial design and has been shown to be sufficient to describe the majority of steadystate process responses. Hence in this study, it was decided to use CCD to design the experiments. Hence the total number of tests required for the three independent variables is 23 + (2x3 + 6 = 20. Once the desired ranges of values of the variables are defined, they are coded to lie at Âą1 for the factorial points, 0 for the center points and Âąp for the axial points. 3.4 Factors and Levels In this study three parameters have been chosen for analysis. They are welding speed, welding current and gas flow rate [34, 12]. Several trial runs were conducted to determine the range of parameters. The levels for parameters finally chosen are shown in table 2.
231  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236 Table 3: central Composite Design Matrix Gas flow Exp Welding speed Welding rate No. (mm / min) current ( A) ( LPM) 1. 1 1 1 2. 1 1 1 3. 1 1 1 4. 1 1 1 5. 1 1 1 6. 1 1 1 7. 1 1 1 8. 1 1 1 9. 1 0 0 10. 1 0 0 11. 0 1 0 12. 0 1 0 13. 0 0 1 14. 0 0 1 15. 0 0 0 16. 0 0 0 17. 0 0 0 18. 0 0 0 19. 0 0 0 20. 0 0 0 Table 4: Experimental Design Variables Welding Welding Gas flow Exp speed current rate No. ( mm / min) (A) (LPM) 1. 150 100 10 2. 200 100 10 3. 150 120 10 4. 200 120 10 5. 150 100 12 6. 200 100 12 7. 150 120 12 8. 200 120 12 9. 150 110 11 10. 200 110 11 11. 175 100 11 12. 175 120 11 13. 175 110 10 14. 175 110 12 15. 175 110 11 16. 175 110 11 17. 175 110 11 18. 175 110 11 19. 175 110 11 20. 175 110 11
4. EXPERIMENTAL WORK 4.1 Experimental Procedure Welding specimen has been prepared to fabricate TIG welded joints. Aluminium alloy 65032 specimen (75mm x 75mm x 3mm) in the specified dimension was considered for welding of square butt joints.
Welding process has been carried out in TIG welding machine. Experiments were conducted based on central composite design matrix [5] which is given in Table 4.
Fig. 1 Photos of Welded Specimen 4.2 Tensile Testing The ultimate tensile strength of the machined specimen were tested in the calibrated universal tensile testing machine. Percent elongation was also calculated. Tensile test carried out according to ASTM standards, using specimen prepared as shown in Fig.2
Fig.2 Dimensions of tensile test specimen 4.2.1 Test Specimen Welded joints were machined for conducting tensile test. Test specimen prepared according to ASTM Standards is shown in Fig 3.
Fig.3 Test Specimen The Tensile test was carried out in the servo controlled universal testing machine with 1000 KN load capacity. The specimen is loaded at the rate of 0.1KN/Min. Due to the pulling effect of machine, tensile specimen undergoes deformation. Twenty specimens were tested at each condition,
232  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236 ultimate tensile strength and percent elongation were calculated
Fig.4 Specimen after tensile test Table 5:. Tensile strength and % Elongation values Gas Welding Welding Tensile Exp. Flow % Speed Current Strength No Rate Elongation (Mm/Min) (Amps) (Mpa) (Lpm) 1 150 100 10 112.7 6.12 2 200 100 10 98.6 5.8 3 150 120 10 109.3 6.1 4 200 120 10 88 5.55 5 150 100 12 122.6 6.25 6 200 100 12 95.7 5.6 7 150 120 12 112 6.15 8 200 120 12 93.3 5.7 9 150 110 11 117.3 6.20 10 200 110 11 100.8 5.9 11 175 100 11 93.3 5.65 12 175 120 11 98.6 5.85 13 175 110 10 104 5.95 14 175 110 12 93.6 5.65 15 175 110 11 96 5.75 16 175 110 11 96 5.75 17 175 110 11 93 5.6 18 175 110 11 96 5.7 19 175 110 11 90.6 5.55 20 175 110 11 96 5.75
5. RESULTS AND DISCUSSION 5.1 Analysis of variance Analysis of variance (ANOVA) is similar to regression in that it is used to investigate and model the relationship between a response variable and one or more independent variables. In this study general linear model is used to determine the influence of welding speed, current and gas flow rate on ultimate tensile strength and % Elongation.
Contribution (%) Regression 9 1465.6 1465.6 6.55 0.004 85.49 Model Linear 3 999.83 999.83 13.40 0.001 58 Square 3 452.52 452.52 6.07 0.013 26.39 Interaction 3 13.25 13.25 0.18 0.909 0.77 Residual 10 248.64 248.64 Error Lack of Fit 5 222.24 222.24 8.42 0.018 12.96 Pure Error 5 26.4 26.4 Total 19 1714.24 100 Source
DF SS
MS
F
P
5.3 Model coefficients for UTS. Table 7 Term Coef Term Coef Term Coef Constant Welding Welding 96.138 speed*welding 10.6045 speed*welding 0.1250 speed current Welding Welding Welding speed 9.75 current*welding 2.4955 speed*gas 1.2750 current flow rate Welding Welding Gas flow rate current 2.17 0.3545 current*gas 0.1250 *gas flow rate flow rate Gas flow 0.46 rate Table 6 shows ANOVA table corresponding to ultimate tensile strength. Linear has great percentage of contribution on UTS and Interaction has less percentage of contribution on UTS. Table 7 shows estimated model coefficients for ultimate tensile strength. 5.4 Estimated regression Model for UTS From Regression analysis, a mathematical model for predicting UTS in terms of welding speed, current and gas flow rate is developed and is given below. UTS = 96.138 – 9.75 x S – 2.17 x I + 0.46x L + 10.6045 x S2 – 2.4955 x I2 + 0.3545 x L2 + 0.1250 x S xI – 1.2750 x S x L + 0.1250 x A x L. 5.5 Analysis of variance for % Elongation Table 8: ANOVA For %Elongation S = 0.1397, Rsq = 80.0% Rsq (adj) = 75.21%
5.2 Analysis of variance for UTS Table 6: ANOVA For UTS S = 4.986, Rsq = 85.5% Rsq (adj) = 75.1%
233  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236
8.86 0.004 52.37
Square
3
0.24406 0.081
4.17 0.037 24.74
0.01584 0.0052
0.27 0.845 0.0162
10 0.19509 0.019



Lack of Fit 5
0.15675 0.031
4.09 0.047 
Pure Error 5
0.03833 0.007

Total
19 0.97366 


Predicte d Respons e
Gas flow rate 11.9 122. 122. 88 119.1298 9 6 6 Upper
0.51867 0.1728
Target
3
Residual Error
Optimum Combination Para Go Weldi meters al ng speed Tensile Ma 108.38 150 strength x 5 % Ma 108.38 Elongat 150 x 5 ion
Lower
Linear
Interaction 3
Table 10: Response optimization for process parameter
Curren t
Contribution Source DF SS MS F P (%) Regression 9 0.77857 0.86508 4.43 0.015 80.4 Model
11.9 5.5 6.25 6.25 6.21 9 5
100
5.6 Model Coefficients For Percent Elongation. Table 9 Term Coef Term Coef Constan Welding t 5.730 speed*welding 0.2486 speed Welding Welding speed 0.227 current*weldin 0.05136 g current Welding Gas flow rate current 0.017 *gas flow rate 0.00136 Gas flow
Term Welding speed*weldin g current Welding speed*gas flow rate Welding current*gas flow rate
Coef 0.00375 0.2875
0.03375
0.007 Table 8 shows the ANOVA table corresponding to % Elongation. This table shows that main effects of welding speed, current and gas flow rate are all significant with respect to percent elongation. Table 9 shows estimated model coefficients for percent elongation. 5.7 Estimated Regression model for % Elongation %Elongation = 5.730 – 0.227 x S  0.017 x I – 0.007 x L + 0.2486 x S2  0.05136 x I2  0.00136 x L 2 0.00375 x S x I – 0.2875 x S xL + 0.03375 x I x L. 5.8 Optimization of process Parameters One of the most important aims of experiments related to welding is to achieve high value of tensile strength and Elongation. The response surface optimization is a technique for determining best welding parameter combination[67,13]. Here the goal is to maximize UTS and % Elongation. RSM optimization result for UTS and % Elongation is shown in Fig 5. Optimum parameters obtained are shown in table 1
Fig 5. Optimization using MINITAB VI4 Software 5.9 Effect of process parameters on UTS The main effects of the plot, for UTS with the process parameter of welding speed, current and gas flow rate were shown in Fig.5.2. Graph shows that UTS decreases from 115 MPa to 95 MPa. when welding speed increases from 150mm/min to 200 mm/min,because of less penetration depth. UTS decreases from 105 MPa to 101MPa when current changes from 100 Amps to 120 Amps, due to the result of increased input heat associated with the use of higher current. As gas flow rate changes from 10 LPM to 12 LPM,UTS increases from 103Mpa to 104Mpa,due to decrease in the porosity level of weld metal. Fig 7 is contour plot, is a graphic representation of the relationship among three numeric variables in two dimensions
Fig.6 Main effect plot for UTS
234  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236 6. CONCLUSION
Fig.7 Contour plot for UTS 5.10 Effect of Process parameters on Percent Elongation The main effect plot shows that value of percent elongation decreases as welding speed increases from 150mm/min to 200mm/min. it is due to the fact that orientation of the grains has the predominant effect on the decreased ductility with increasing travel speed. As current changes from 100A to 120 Amps, percent elongation decreases due to high heat input. When gas flow rate increases from 10 LPM to 12 LPM,percent elongation decreases. Fig. 9 shows the contour plot for percent Elongation at Constant welding speed, current and gas flow rate.
The effect of TIG welding parameters like welding speed, current and gas flow rate on ultimate tensile strength and percent elongation in welding of Al65032 has been studied. Experiments were conducted using central composite design matrix and mathematical models have been developed. From the study it was observed that welding speed has the most significant effect on both UTS and percent Elongation followed by welding current. However gas flow rate has least significant influence on both UTS and percent elongation. Optimization was done to maximize UTS and percent elongation. Predicted properties at optimum condition are verified with a confirmation test and are found within the limits.
REFERENCES [1]
[2]
[3]
[4]
[5]
Fig. 8 Main effects plot for percent elongation [6]
[7]
[8]
G.Hargopal, P.V.R.Ravindra reddy, “Parameter design for MIG welding of Al65032 alloy using Taguchi technique”, Journal of scientific and industrial research, vol 70,2011,pp.844850. G.Padmanaban, V.Balasubramanian, “Optimization of pulsed current gas tungsten arc welding process parameters to attain maximum tensile strength in AZ31B magnesium alloy”, Trans.Non ferrous Met.soc.china 21,2011,467476. R.Satish, B.Naveen, “Weldability and process parameter optimization of dissimilar pipe joints using GTAW”.International Journal of Engineering research and applications, vol2,2012, pp.I25252530. Dr.P.Kunar, Dr.K.P.Kohle, “Process optimization of pulsed GTAW process for Al7039 alloy using Ar+He Gas “,IE(I) JournalMC vol 9,2011. Narongchai Sathavornvichit,et al “Central composite design in Optimization of the factors of automatic flux cored arc welding for steel ST37”Regional conference on mathematics, university sains,Malaysia,june 1315,2006. Ugur Esme, Melih Bayramoglu, “Optimization of weld bead geometry in TIG welding process using grey relation analysis and taguchi method”, Original scientific article MTAEC9, 43(3),2009,pp 143149. M.Balasubramanian,V.Jayabalan,“Predictio n and optimization of Pulsed current gas tungsten arc welding process parameters to obtain sound weld pool geometry in Titanium alloy using lexicographic method”,JMEPEG 18,2009,pp 871877. Erdal Karadeniz, Ugur Ozsarac, “The effect of process parameters on penetration
Fig 9. Contour plot for % Elongation
235  P a g e
Palani.P.K, Saju.M / International Journal of Engineering Research and Applications (IJERA) ISSN: 22489622 www.ijera.com Vol. 3, Issue 2, March April 2013, pp.230236 [9]
[10]
[11]
[12]
[13] [14]
[15]
in gas metal arc welding process”, Materials and designs 28,pp 649656,2007. D.S.Nagesh, G.L.Datta, “Prediction of weld bead geometry and penetration in shielded metal arc welding using artificial neural network”, Journal of material processing technology, 123,pp 303312,2002 P.K.Palani, N.Murugan, “optimization of weld bead geometry for stainless steel claddings deposited by FCAW” Journal of material processing technology,vol 190,2007,pp.291299 P.K Palani, N.Murugan, “Modeling and analysis of pitting corrosion resistance of stainless steel overlays deposited by Flux cored arc welding”. Journal of surface engineering, vol 24, 2008, pp 422430. B.Chan, J.Pacey, “Modelling gas metal arc weld geometry using artificial neural network technology”, Canadian metallurgical quarterly, vol 38, 1999. Parmer R.S., Welding Engineering and Technology, Khanna publishers,1997. P K Palani, N Murugan, “Prediction of Delta ferrite content and effect of welding process Parameters in claddings by FCAW.Materials and Manufacturing processes”, 21:431438,2005. P.K.Palani, N.Murugan, “Development of mathematical models for prediction of Weld bead geometry in cladding by flux Cored arc welding”. Int J Adv Manuf Technol ,2006, 30: 669676
236  P a g e